Silica is the second abundant element in the biosphere and many organisms utilize it as a structural component (Rupcich
Silaffin is a protein from in diatoms and is known to facilitate the silica synthesis (Kröger
Sericin is a minor protein that is secreted by the silkworm. It bonds two brins of fibroin fiber together and make able to maintain the shape of cocoon. Sericin is usually discarded by the degumming process but could be used as new source of biopolymer, because it is easy to extract and able to get in large quantities. Currently sericin is used as an ingredient of cosmetics (Kim
Silk cocoon was obtained from Hung Jing Co., LTD. (Seoul, Korea). All other chemicals were purchased from Sigma-Aldrich LTD. (Yongin, Korea).
Silk cocoons were boiled with distilled water using an autoclave at 120℃ for 1 h. The solution was filtered with a nonwoven filter in order to remove the remaining silk fibers. The solution was freshly made every time before the experiment. The final concentration of sericin was 1 %(w/v).
The synthesis of silica was performed by mixing tetraethyl orthosilicate (TEOS) and sericin solution. More precisely, 500 µL of TEOS and 500 µL of sericin solution were added in a Eppendrof tube, and it was shaken vigorously with an orbital shaker. The tube was incubated at room temperature without further stirring. After 1 wk, 400 µL of ethanol was added to the mixture and centrifuged at 10,000g for 1 min in order to precipitate the reactant. The precipitate was further washed with ethanol 3 times. The collected precipitate was dried in a vacuum chamber for 36 h in order to remove residual ethanol.
The formation of silica was verified by thermal gravimetric analysis (TGA, Q-5000 IR, TA-Instrument, USA), Fourier transformed-infrared spectrometer (FT-IR, MIDAC, Japan) and 29Si nuclear magnetic resonance spectrometer (NMR, AVANCE, Bruker, Germany). The heating rate of TGA was 10℃/min and the data in the range of 100-600℃ were collected under nitrogen gas purging. In the case of FT-IR, the spectrum was obtained from KBr method after 24 scans and the resolution was 4 cm-1. Solid-state 29Si MAS NMR spectra were acquired on a DSX- 400 NMR spectrometer (Bruker, Germany) operating at 79.5 MHz. Detailed conditions were as follows: spinning rate, 3.5 kHz; pulse length, 4.2 μs; recycle delay, 30 s. Field emission scanning electron microscope (FE-SEM, SUP-RA55 VP, Carl Zeiss, Germany) was employed to observe the microscopical morphology of the precipitate.
We prepared sericin solution by the hot-water extraction method. Sericin solution was added to TEOS and left in the chamber without stirring for 1 wk at room temperature. The TEOS and the sericin solution did not mix each other (Fig. 1a), and a white precipitate was formed only at the interface between the TEOS and the sericin solution. In order to improve the precipitation, we stirred the reaction tube vigorously. A dispersion of the two liquid was formed in the sericin layer and maintained through the incubation time. The white precipitate was grown in the sericin solution layer during 1 wk of incubation (Fig. 1b). Fig. 1c shows the final precipitate obtained after washing and drying.
In order to verify the synthesis of silica, we first performed TGA analysis. While sericin decomposes over 200℃, the weight loss of precipitates was about 15% even at 600℃ indicating the formation of silica (Fig. 2). In the case of the precipitate, there was a significant loss of weight between 200~400℃ which was the same temperature range that the thermal degradation of sericin occurs. Therefore, the precipitate might be a complex of silica and sericin. Based on the TGA results, the weight percent of silica and sericin in the complex would be 87 and 13%, respectively.
The formation of silica-sericin complex could be also verified by the ATR-FTIR results (Fig. 3). The asymmetric stretch, symmetric stretch and bending vibration of Si-O-Si at 1100, 800 and 450 cm-1, respectively, could be observed in the ATR-FTIR spectrum (Siuzdak
The synthesis of silica can be also verified by the NMR. Generally, Q
Quantitative analysis of Q2, Q3, and Q4 peaks in silicasericin complex.
Fig. 5 shows the FE-SEM image of silica-sericin complex. It had a fractal structure where sphere-like particles having tens of nanometer size are agglomerated into large and irregular shapes.
Generally, TEOS is hydrolyzed under acidic or basic condition to in order to synthesize silica through sol-gel process. However, the present study shows that silica could be synthesized directly from TEOS without any hydrolysis. It seems that the role of sericin during silica formation is similar to silicatein. Further application of the synthesized silica nano- and microparticles in biomedical field is under investigation. Expected area is drug delivery and tissue engineering where silicatein is currently applied (Schröder